Guide to de-rusting and coating metal fuel tanks
Download 28.77 Kb.Pdf ko'rish
- Bu sahifa navigatsiya:
- Please read the whole of these instructions before starting work. If you follow them correctly you
- Thoroughly flush the tank with water
- De-rusting and corrosion protection 1
- The solvent is volatile as so it is important to stress that this air supply must not come from an electrical appliance that
- After this 30 minutes, with the tank still in the same position
- With the tank still upside down and the
A guide to de-rusting and coating metal fuel tanks.
Congratulations, you’ve bought a product
that will protect your tank against all petrol
mixes up to and including 100% ethanol
starting work. If you follow them correctly you
will get a perfect result. If you do not follow them
the result will be different!
Time and temperature are important to complex
De-rusting and Coating Fuel Tanks
Fuel tanks made from steel are susceptible to rusting. In the
past when leaded fuels were in use, the problem was greatly
minimised. As unleaded petrol is now used for health and
environmental reasons older vehicles and engines have to cope
with it. The availability of leaded petrol has been vastly reduced
all over Europe.
Unfortunately modern fuels, even with an oil mix for two stroke
engines, are aggressive to such an extent, that steel tanks corrode
even when full. This is caused by the added MTBE (methyl-
tertiary-methyl–ether), which is being increasingly added to
improve the anti knock performance of the petrol.
The best preventative and remedial measure is Tapox, a 2 part
epoxy which is designed specifically to be resistant to fuel and
maintain a corrosion free tank..
If the tank is suffering from corrosion the instructions below
show how to eliminate corrosion completely.
If your tank already has a lining that is damaged and needs
removing we can supply our specially designed product
SEALEREATER which will remove it.
Fedox Rust Remover
which will remove any amount of rust from a
tank and leave you with a bright grey surface. Good for cleaning
Fertan Rust Converter which will convert rust to a safe and permanent
coating of iron tanate and zinc phosphate. Good to use in a tank but the
best product for all other corrosion situations where it can be applied by
brush, spray or roller.
With the tank removed from the vehicle ensure it is completely empty of
fuel. Please dispose of remaining fuel in an appropriate manner or store
for later use.
Rinse the tank with plenty of water.
Close the petrol cock and / or seal any connections. Pour about 50cc of
washing up liquid into the tank and add warm water. Leave this solution
in the tank for about an hour, agitating the tank to thoroughly clean all
inside surfaces. Drain the cleaning fluid and dispose of appropriately.
If your tanks have an existing liner then that can be removed now with
SEALEREATER as a first step. Then repeat the washing before moving
on to the stage below. Obey the care instructions.
Now, fill the tank with approx. ½ to 1 litre of FERTAN‘s (or other)
alkaline engine cleaner. Please do not use a mineral based product.
Petrol, acetone, thinners or degreasing agent are also not suitable. Again
seal all connectors and shake thoroughly to dissolve any remaining oil
and petrol within the tank.
Leave cleaner to work for at least 1 hour agitating frequently and then
empty the tank into a suitable container. If the cleaning fluid is not too
contaminated re-use it at a later stage for cleaning the engine / gear box/
back axle. It may be useful to filter the cleaning fluid, coffee filter paper
can be used.
facilitate complete drainage.
To accelerate the treatment with FERTAN Rust Converter, luke warm
water can be used for the final rinse.
You should wear rubber gloves /
household gloves for
these and the following procedures.
If you are flushing the tank in a sink put the tank on a soft surface. This
prevents damage to ceramic sinks and to the fuel tank. When disposing
of the rinse, do not drain it onto light coloured brick as it has a bleaching
Do ensure and check that the tank is drained completely and then screw
the connectors back on, sealing the tank. The petrol tap, if fitted, should
be moved to the ‘closed ‘position.
Now you need to decide whether the inside of the tank, in addition to
degreasing, needs to be taken back to bare metal, or whether the
appearance of the surface after applying the final coat is less important to
To just treat the rust only Fertan Rust Converter is required.
This is not a quality issue, just one that may effect the smoothness of the
If you use Fedox follow the mixing instructions on the bottle. The Fedox
will completely lift and eliminate any rust in the tank. After rinsing out
the Fedox and rust the bare metal surface should be protected against
new corrosion by Fertan Rust Converter.
Pour FERTAN Rust Converter into the tank which should still be damp
from the final rinse. Use about 0.25 litres for a 10 – 15 litre tank
volume, 1 litre in a 40 – 50 litre tank. More may make the job of coating
the inside of the tank easier but it is more costly.
Now turn and shake the tank with FERTAN Rust Converter ensuring
that the inside of the tank is completely covered by the fluid. Particular
attention should be paid to slanting areas such as frame mountings, here
it is important to shake the tank well to ensure that even difficult to reach
areas are completely covered. It may be advisable to leave the tank
laying in several different positions to ensure thorough coverage.
Then completely drain the FERTAN Rust Converter from tank into
clean plastic container.
Remove all seals from the tank and store it for a minimum of 24 hours at
a temperature of 20 degrees Celsius. This will enable FERTAN to have
its chemical reaction with the metal and ferrous oxides in the tank.
Refill the tank with the previously drained amount FERTAN, re-fit
connectors etc. and shake tank thoroughly to enable even coverage and
then fill up the tank with clean warm water. Leave the mixture
(FERTAN/water) to work overnight (12 hours) at room temperature.
Finally drain the tank and rinse thoroughly to remove any loose particles
and leave to dry. Hair-dryer comes in useful.
At this stage any petrol caps/ connectors, petrol cocks etc. must be
cleaned and rinsed immediately with clear water. Any FERTAN
splashes on the exterior of the tank must be wiped immediately by
sponge and water to avoid discolouring the paint work. This is not less
important if the tank has been painted recently.
Although this method may seem to be labour intensive and time
consuming, it ensures that the tank is completely de-rusted and
avoids the unnecessary removal of material caused by mechanical
de-rusting processes. This means the tank has not been weakened as
happens with bead blasting or grinding. And it only takes 15
minutes actual work.
Protection 2 - components
Now, we are ready to use the fuel resistant
Tapox coating. This is going into an absolutely
rust-free tank and will reliably prevent any future
Later in this process it is necessary to ensure ventilation after
coating the inside of the tank Only a very gentle supply of air
is required (approx. 0,2 – 0,4 bar max) preferably from a
compressor, though only a small air supply is required. The
constant air movement will accelerate the drying process in the
tank itself. Moving air removes the solvent quickly and
prevents solvent entrapment and/or the coating moving inside
the tank before it dries.
The solvent is volatile as so it is important to stress that this
air supply must not come from an electrical appliance that
could spark as the evaporating solvent could catch fire.
Keep away from open flames – No smoking and ensure
(We use either a normal air compressor with the flow reduced to a trickle
or the cheapest 12v airbed inflator from Tesco)
The coating of the tank interior will be the TAPOX, which has to be
mixed before the coating begins with hardener T X 10.
Find a paint whisk to go in an electric drill. Remove the lid from the big
can and drill a hole for the shaft of the whisk.
To start the reaction add the entire contents of the smaller can of
hardener (Component 1) into the coating (Component 2) and mix
thoroughly at slow speed for 3 minutes using a small whisk. You can
mix by hand but please ensure complete mixing.
This Tapox mix is sufficient for tanks of 15 - 20 litres and the solution
may be mixed in the supplied can (750 ml).
Ensure all tank openings are sealed excepting the filler. The tank is dry
and rust-free after de-rusting and coating treatment with FERTAN, so
the mixed TAPOX can now be poured into the tank filler neck Firmly
lock the filler neck It would be advisable to put a thick plastic cover
under the tank cap if the original cap is used, this would avoid
Now turn the tank on its side and up side down etc. to ensure thorough
coating from all angles. Shake to cover any baffles. After 2 or 3
minutes of this open the petrol cap and drain all remaining liquid into the
TAPOX container. Now open the hole used by the petrol connector.
You must ensure that all residue is properly drained off. Any splashes
that have occurred on the exterior paint must be immediately wiped off
with thinner (Nitro/Universal - thinner)
constant air flow through the petrol connector opening into the tank for a
minimum of 180 minutes so that all solvent residue is expelled. It is
heavier than air. This process is complete as soon as the coating inside
of the tank is dry. If the tank has ¼” internal screw thread (internally or
externally) an air coupling may be firmly attached for connection
purposes, which makes this process considerably easier.
It is of great importance that the air passing through the tank has is low
pressure, a maximum of 0,2 – 0,4 bar otherwise the coating, still soft at
this stage, could be damaged. (Compressor or air bed inflator)
(The coating fluid that was drained from the tank be thrown away or
used for any other job as a coating. It will store at 4 degrees Celsius for
up to 12 hours).
lowest point downwards leave the tank sealer to harden off. Minimum
time is 6 days (144 hours) at 20C. Both the temperature and the time is
Electric drill (pref.)
Download 28.77 Kb.
Do'stlaringiz bilan baham:
ma'muriyatiga murojaat qiling